O SlideShare utiliza cookies para otimizar a funcionalidade e o desempenho do site, assim como para apresentar publicidade mais relevante aos nossos usuários. Se você continuar a navegar o site, você aceita o uso de cookies. Leia nosso Contrato do Usuário e nossa Política de Privacidade.
O SlideShare utiliza cookies para otimizar a funcionalidade e o desempenho do site, assim como para apresentar publicidade mais relevante aos nossos usuários. Se você continuar a utilizar o site, você aceita o uso de cookies. Leia nossa Política de Privacidade e nosso Contrato do Usuário para obter mais detalhes.
A Scribd passará a dirigir o SlideShare em 1 de dezembro de 2020A partir desta data, a Scribd passará a gerenciar sua conta do SlideShare e qualquer conteúdo que você possa ter na plataforma. Além disso, serão aplicados os Termos gerais de uso e a Política de Privacidade da Scribd. Se prefira sair da plataforma, por favor, encerre sua conta do SlideShare. Saiba mais.
Manufacturing Technology II
Dr. Chaitanya Sharma
PhD. IIT Roorkee
In this chapter we shall discuss the following:
Solidification of casting
Functions of riser
Types of riser
Methods for riser design
1. Look up
2. View Slides;
3. Read Notes,
4. Listen to
Keywords: Solidification shrinkage, Cooling characteristics,
Freezing ratio, modulus, NRL method
Solidification of Casting
• During solidification metal experience shrinkage which
results in void formation.
• This can be avoided by feeding hot spot during
• Riser are used to feed casting during solidification.
Solidification of Iron & Carbon
Figure 10.5 (a) Solidification patterns for gray cast iron in a 180-mm (7-in.) square casting. Note that
after 11 minutes of cooling, dendrites reach each other, but the casting is still mushy throughout. It takes
about two hours for this casting to solidify completely. (b) Solidification of carbon steels in sand and
chill (metal) molds. Note the difference in solidification patterns as the carbon content increases.
What Are Risers?
• Risers are added reservoirs designed to feed liquid
metal to the solidifying casting as a means for
compensating for solidification shrinkage.
• Riser must solidify after casting.
• Riser should be located so that directional
solidification occurs from the extremities of mold
cavity back toward the riser.
• Thickest part of casting – last to freeze, Riser should
feed directly to these regions.
• The shrinkage occurs in three stages,
1. When temperature of liquid metal drops from Pouring
to Freezing temperature
2. When the metal changes from liquid to solid state,
3. When the temperature of solid phase drops from
freezing to room temperature
• The shrinkage for stage 3 is compensated by providing
shrinkage allowance on pattern, while the shrinkage
during stages 1 and 2 are compensated by providing
Solidification Time For Casting
• Solidification of casting occurs by loosing heat from the
surfaces and amount of heat is given by volume of
• Cooling characteristics of a casting is the ratio of
surface area to volume.
• Higher the value of cooling characteristics faster is the
cooling of casting.
Chvorinov rule state that solidification time is inversely
proportional to cooling characteristics.
Ts = Solidification time V = Volume of casting
SA = Surface area K = mould constant
• A cylindrical riser must be designed for a sand-casting
mold. The casting itself is a steel rectangular plate
with dimensions 7.5 cm x12.5 cm x 2.0 cm. Previous
observations have indicated that the solidification
time for this casting is 1.6 min. The cylinder for the
riser will have a diameter-to-height ratio as 1.0.
Determine the dimensions of the riser so that its
solidification time is 2.0 min.
• V/A ratio = (7.5 x 12.5 x 2) / 2(7.5x12.5 + 12.5x2 +
7.5x2) = 187.5 / 267.5 = 0.7
Methods of Riser Design
• Following are the methods for riser design:
1. Caine’s Method
2. Modulus Method
3. NRL Method
• Caine’s equation
X = Freezing ratio
Y = Riser volume / Casting volume
A, b and c = Constant
Constant For Caine’s Method
• Values of constants are given in table:
Modulus is the inverse of the cooling characteristic ( surface area/
Volume) and is defined as
Modulus = Volume / Surface area
In steel casting riser with height to diameter ratio of 1 is generally
Volume of cylindrical riser =
Surface area =
For sound casting modulus of riser should be greater than the
modulus of casting by a factor of 1.2. Therefore Mr = 1.2 Mc
On simplification D = 6 Mc
Considering contraction of metal
• NRL stand for Naval research Laboratory.
• NRL method is essentially a simplification of Caine’s method.
• In this method shape factor is used in place of freezing ratio.
• Ratio of riser volume to casting volume can be obtained from
graph shown below.
• After obtaining riser volume riser diameter and height can be
• Use H/D = 1 for Side riser and H/D =0.5 for Top riser
Example:2 Design a suitable
riser for the given casting
Solution: Neglecting branch first calculate shape factor
Shape factor = (Length + Width)/ Thickness
= (25+ 12.5)/5 =7.5
Volume of casting VC = 25 x 12.5 x 5
= 1562.5 cm3
Volume of riser VR = 0.575 x VC
= 0.575 x 1562.5
= 898.43 cm3
Volume of riser VR = 2.5 x 2.5 x 10
= 1562.5 cm3
This is a plate feeding bar with a thickness ratio of 0.5,
hence from figure 4.30 (PN Rao), we get parasitic volume
as 30 %
Hence riser volume = 0.30 x 62.5 + 898.43 = 917.2 cm3
Riser diameter D = 10.53 cm
• Choke area is the main control area which meters the metal
flow into mould cavity.
• Normally choke area happens to be at the bottom of the
sprue so sprue should be designed first.
• Having sprue bottom as the choke area help in establishing
proper flow in the mould easily and early.
• Choke area can be calculated by Bernoulli’s equations
• Q= AV
• W =ρAV
• Choke area A = W/ ρV
= W/ ρ√2gH
= W/ ρ t c √2gH
Effective Sprue Height
• Effective sprue height H, of a mould depends on the
casting dimensions and type of gating system.
• It can be calculated using following relations:
h =Sprue height
p = Height of mould cavity in cope
c = Total height of mould cavity
Values of h, P and c are shown in for various gating system
• Time required for filling a mould is pouring time.
• Too long pouring time – Higher pouring temperature
• Too less pouring time – Turbulent flow & defective
• It depends on casting material, complexity of casting,
section thickness and casting size.
• Pouring time is calculated by empirical formulas obtained
by experiments which differ from one material to
another and one casting to other.
• For non ferrous material, long pouring time would be
beneficial since they lose heat slowly and also tend to
form dross if metal is poured too quickly.
Grey cast iron, mass less than 450 kg
Grey cast iron, mass greater than 450 kg